Tribology in Industrywww.tribology.rs
Effect of Heat Treatment on Wear behavior of
Hybrid Aluminum Metal Matrix Composites
aSJM Institute of Technology, Chitradurga, Karnataka, India, bUniversity BDT College of Engg, Davangere, Karnataka, India, cJain Institute of Technology, Davangere, Karnataka, India.
Dry sliding wear Age hardening Taguchi’s DOE ANOVA
A B S T R A C T
The focus of the paper is the wear behavior of hybrid aluminum metal matrix composites. The main objective of the investigation is to conduct the wear test at room temperature for both the as-cast and age hardening conditions. Materials chosen for the study are Aluminum 7075 as a matrix, Silicon Carbide and Alumina are the reinforcements. Hybrid metal matrix composites are produced by utilizing stir casting route for 5–15 wt.% silicon carbide and alumina. Microstructural characterization of hybrid aluminum metal matrix composites reveals the homogeneous mixing of reinforcements. It is noticed that the higher composite hardness is obtained due to the raise in weight percentage of the reinforcement up to 10% of hybrid reinforcements. In the T6 heat treatment, there is a gain in hardness by 24 % for optimum percentage of reinforcement i.e. 10 % compare with as-cast composites.
© 2019 Published by Faculty of Engineering
SJM Institute of Technology, Chitradurga, Karnataka, India E-mail: email@example.com
Aluminum matrix composites (AMC) is the largest gathering of MMCs. AMCs are normally based on aluminium-silicon compounds and on the combinations of series 2000 and 6000 series. AMCs are reinforced by Al2O3 (Alumina) or SiC
(silicon carbide) particles in proportions of 03-20 wt% might be as long/short fibres and/or particles of Al2O3, SiC, Graphite. AMCs can be
prepared by Powder metallurgy (sintering); Stir casting; Infiltration methods. High strength even at raised temperatures, high load/deformation, low density, high thermal conductivity, increased wear resistance behavior  are the
some of the properties of AMCs. Hybrid aluminum metal matrix composites (HAMMC) materials are an excellent substitute to conventional materials, because of the enhanced hardness, specific strength and creep resistance properties. Based on these properties, one can consider the HAMMC for the automobile and aerospace applications .
A surface phenomenon referred as wear will occurs by relocation & separation of material. It generally suggests a progressive loss of material and change of measurements over some undefined time frame. The main components that influences wear and friction
behavior of aluminum alloys are sliding distance and speed, normal load, frictional temperature, surface finish and contaminants, hardness, microstructure etc.
Singla et al.  developed aluminium alloy/ SiCp
composites of varying weight fractions of silicon carbide (5-30 %) by stir casting techniques using a two step-mixing method. Al-SiCp was
tested to find the impact strength and hardness. From the results, it can be shown that impact strength and hardness increases with increment in weight percentage of reinforcement.
K. Ravi et al.  investigated the Al-fly ash composite prepared by utilizing stir casting method. Al-fly ash particles with 3-12 wt.% and different particle size are used to determine the dry sliding wear behavior for different loading, sliding speeds in pin-on-disc experiment. Outcomes of the experiments shows that composite materials reinforced with coarse particles of fly-ash demonstrate greater resistance to wear than fine particles of fly-ash. Komai et al  conducted the experimentation to determine the mechanical properties of Al7075-SiC composite. From the result, it is observed that the better mechanical properties of A7075-SiC whiskers composite have been obtained. Rupa Dasgupta et al.  conducted experimentation to find the wear behavior and hardness of the A7075-SiC composite. From the outcomes, it is confirmed that the enhancement in hardness, wear resistance properties are obtained.
R.L. Deuis et al.  surveyed the wear behaviour of the materials and the development of fine equiaxed wear debris is related with a stable tribo-layer on the worn surfaces. The critical parameters for adhesive wear are applied load, sliding velocity, the surface hardness of worn surface and morphology in relative to the theories of wear encuontered by the materials. In this audit current wear hypotheses, issues identified with counter face wear, and wear systems are talked about.
V.C. Uvaraja et al.  studied wear behavior of Al6061 and Al7075 alloy with SiC and B4C
reinforcements. From the results obtained from the experiment it is concluded that the enhanced wear rate and hardness of Al7075 hybrid metal matrix composites was found as compared to Al6061 hybrid metal matrix composites.
Radhika et al. [10-11] has conducted the experiments to evaluate the wear characteristics of Al/Gr/Al2O3 hybrid MMC and suggested that
the graphite reinforcement has boost up the resistance to wear. This increment is due to the forming a protective layer between the counterface & pin. Addition of the reinforcement Al2O3 has considerable influence in reducing
wear rate of the composite
Saleemsab Doddamani et al.  conducted experimentation on wear behaviour of Aluminum-graphite MMC. From the results it is found that the adding of particles of graphite has increased the resistance to wear of the MMC. Also it is reported that addition of particles of graphite in aluminum reduces the friction then that of the base alloy.
Rajesh AM et al. [13-15] conducted experimentations like hardness, wear behavior at as-cast and age hardened conditions etc on aluminum hybrid metal matrix composites. The matrix material considered is Al7075, and reinforcement material is SiC and alumina. From the results it is clear that the HAMMCs have better properties as compared to unreinforced aluminum alloy.
Mouritz et al.  reported changes of resistance to abrasive wear of aluminium matrix composite when subjected to the various aging environment. In aged conditions, composite materials exhibits relatively high wear resistance.
N. Radhika  studied abrasive wear behavior of cast aluminum-SiC composite with nickel coating. For the study of wear behavior they utilized Taguchi design of experiments and Analysis of Variance (ANOVA).
2. EXPERIMENTAL PROCEDURE
It is identified from the literature that more research work has been done on the wear behavior of Al-SiCp, Al-graphite, Al-Fly Ash
MMCs. In the background, hybrid aluminum metal matrix composites have a wide range of scope for the research in wear characterization. The material selected for the research work is Al7075 as matrix and silicon carbide and alumina particles as reinforcement.
The Al7075/SiC/Al2O3 particulate MMCs are
discontinuously reinforced composites which are nearly isotropic  and also have exceptional combinations of tribological and weight reduction properties.
The motivation to utilize Al7075 is the tensile strength of the material which is higher than the any other grades of the aluminum. The main constituents in the Al7075 are Si=0.4 %, Zn = 6.1 %, Mg=2.9 %.
The SiC material is a blend of silicon and carbon, outstanding abrasive material. Now a day, the SiC material is formed into a technical grade better quality ceramic with excellent mechanical/physical properties. Some of the key properties of silicon carbide utilized here are Density – 3.1 g/cc, melting point – 2730 0C, molecular mass – 40.10 g/mol,
particle size=100 µm,, Appearance –Black in color.
The alumina (Al2O3) is corundum. The alumina
as a reinforcement is steadier with aluminum and withstand higher temperatures. Some of the key properties of aluminum oxide utilized here are density=3.69 g/cc, melting point – 2072 0C,
particle size=60 µm, appearance - White in color.
Al7075-SiC/Al2O3 samples are formed at varied
weight fractions of SiC/Al2O3 (5 %, 10 %, and 15
%) utilizing stir casting technique. The aluminum slabs were melted in the furnace as appeared in Fig. 1. In the wake of liquefying, liquid aluminum was superheated to 750 0C temperature.
The required measures of SiC/Al2O3 particles were
added to the liquid aluminum while mixing with a stirrer at 600rpm speed . The liquid
Al7075-SiC/Al2O3 was filled a permanent mold and it was
permitted to set. The Al7075-SiC/Al2O3 composite
bars were taken out from the mold. The samples were set up from as-cast combinations for investigation of required properties.
Fig.1 . Induction furnace.
2.3 Age Hardening
The as-cast composite specimens were heat treated at a temperature of 4650C for 02 hrs taken
after by quickly quenched in cool water. After quenching the specimens, these are subjected to an age (precipitation hardening) by heat-treatment the specimens to 120 0C, maintaining
this temperature for 05 hrs and after that taken after cooling in air to room temperature.
2.4 Hardness Test
The Vickers’ indentation hardness measurement technique comprises of diamond indenter used to indent the test specimens. The diamond indenters used is having square base with pyramid shape and a point of 136o in-between.
The castings are machined to 10mm diameter and 35 mm length for Vickers’ hardness test.
2.5 Experimental Wear Test
6 kg and a fixed velocity of sliding of 0.942 m/s, 1.8849 m/s, 2.82 m/s for 200, 400, 600 rpm respectively for about 5 minutes. The pin specimens are of length 35 mm and diameter 10 mm. Before the wear tests the pins were polished by using emery paper (1000 size grit)
in-ordered to make sure that efficient contact between the flat surfaces and the steel disc. Acetone is used to clean the specimens & wear track. The wear rate is determined by the weight loss method.
A steel disc as conterbody was used, to promote a mechanically mixed layer (MML). It was found from the literature that, the presence of major alloying elements in the Al-alloy that have high solubility in steel promoted a thick mechanically mixed layer. The solubility of Al-alloy elements in Fe is in the order of Si, Mn, Cu, Mg, which roughly approximates the thickness of the MML formed, while the Fe content of the MML also scaled in this order. As for the ceramic material, which also can be used as a conterbody during the wear test, the MML was derived from fracture of the slider, and also from transfer and re-transfer of the aluminium alloy. To analyze the true effect of the work hardening induced by wear, a ceramic slider was used, to minimize the formation of an MML .
2.6 Taguchi’s Optimization
Taguchi method of optimization is one of the most effective techniques because of its simplicity to conduct the design of experiment. The main objective of the Taguchi technique is to evaluate the statistical data which is the input function for optimization. The technique developed for the design of experiments to examine the different parameters and their effect on process mean and variance.
3. RESULTS AND DISCUSSIONS
3.1 Microstructure and EDX Analysis
In the microstructure, shown in Fig. 2, of the Al7075-SiC/Al2O3 particulate composite
confirms uniform distribution of the reinforcement. In the process of the mixing, a whirling of molten material is formed from the rotation of the stirrer through which the SiC/Al2O3 particles are drained into the melt.
(a) As-cast Al7075 (b) 5% SiC/Al2O3
(c) 10% SiC/Al2O3 (d) 15% SiC/Al2O3
Fig. 2. Scanning Electron Micrograph shows a uniform distribution of particles.
The force gave by mixing the molten material with a mechanical stirrer beats the surface vitality hindrance because of poor wettability of SiC/Al2O3
by Al composite. Once the SiC/Al2O3 particles are
moved into the molten aluminum, the dissemination is firmly influenced by certain flow transitions. From the momentum transfer and the outspread flow of melt, lifting of SiC/Al2O3
particles will take place and also causes prevention of particle settling in the matrix. Meanwhile, local hydrodynamic forces are induced on the particle grouping of SiC/Al2O3 particulates.
These forces induced are capable of separating the clustering of SiC/Al2O3 particles which in
turn leads to homogeneous microstructure all through the cast segment. A strong homogeneous microstructure between the reinforcement and matrix helps in the load exchange from the reinforcement to the matrix. Thus, the break happens in the composite via the reinforcement and not along the interface. Despite the fact that the SiC/Al2O3 is a non-load
bearing ingredient, a solid particle/matrix interface helps the SiC/Al2O3 particles install
themselves into the matrix legitimately, enhancing the crack resistance. It has been reported that during solidification, an enhancement in the interfacial relationship between the aluminum matrix and SiC/Al2O3.
By reason of the uniform distribution and good bonding of SiC/Al2O3 particles in the aluminum
matrix, Al7075-SiC/Al2O3 particulate composites
good machinability, low wear rate, high damping capacity, and their outstanding properties.
To determine the chemical composition of the Al7075-SiC/alumina composites, EDX measurements are carried out in the SEM on individual specimens. The EDX analysis indicates the foremost composition of Al7075-SiC/alumina composites silicon, magnesium, Fe, carbon and aluminum. Small amount of oxygen are also observed. The signals of oxygen may arise from the contamination of the aluminum oxide.
Fig. 3. EDX profile analysis for the surfaces: a) 0 % reinforcement, b) 5 % reinforcement, c) 10 % reinforcement, and d) 15 % reinforcement.
Table in the Fig. 3 describes the atom percentage of Si, magnesium, carbon, and aluminum. These outcomes specified that the chemical composition of the Al7075/SiC/alumina is consistent. The atomic percentage of carbon is high than compared to silicon and magnesium. The presence of carbon indicates the adding up of SiC, alumina reinforcement with the Al7075 matrix.
The content of silicon (0.63 to 0.91) and magnesium (0.6 to 2.54) indicates that the presence of Si and Mg in the Al7075 alloy. From the EDX analysis (Fig. 3), it is found that Al7075-SiC/alumina MMCs are rich in both Si and Mg. The existence of MgAl2O4 at interfaces was
confirmed in a detailed study on the interfaces in discontinuously reinforced MMCs. In all the compositions of Al7075-SiC/alumina, oxygen (O) content has been obtained. The content of O is due to the formation of Al2O3 on the top of the
pits as the main compound on the surface.
O- mapping, in addition, is performed to know if any sample of oxidation tested at along with Fe, O was likewise in age hardened Al7075 reinforced with SiC and alumina specimens. The O present in an O2, though, no clarity though it is
an FeO2 or Alumina.
3.2 Micro-hardness Measurement
The Vickers’ indentation hardness measurement technique has been utilized to conduct the experimentation. For each composition of the composite three specimens are utilized. The average of all the results has been considered and displayed in the Table 1.
Table 1. Vickers’ Hardness Number (VHN) for specimens of different composition and conditions.
VHN As-cast Aging
1 Al7075 105 121
2 Al7075/5%SiC&Al2O3 114 131
3 Al7075/10%SiC&Al2O3 116 140
4 Al7075/15%SiC&Al2O3 110 125
hardness number is because of the enlarged bonding area at the interfacial region of the matrix and reinforcement along with grain structure refinement . The standard deviation for the hardness test for as-cast specimens is 3.06 to 4.58 whereas for age hardened specimens it varies from 2.08 to 3.51.
The Fig. 4 shows the effect of the addition of reinforcements on the composite hardness. The evidence is that as percentage of reinforcement is varied by weight, the hardness number of the composites increased monotonically and significantly from 106 to 116 VHN. It is also observed that the hybrid composite with 10 % SiC 10 % alumina shown good hardness property.
Fig. 4. Vickers’ hardness number v/s compositions of specimens for as-cast and age hardened conditions.
Micro-hardness of hybrid composites found incremented with raise in content of reinforcement and enhance in hardness number of Al7075+Al2O3+SiC composites are in the range
of 110-140VHN for with heat treatment. In T6 heat treated, aged HAMMCs the observed hardness was 120, 130, 140 AND 115 respectively for various wt% of SiC and alumina reinforcement in HAMMCs.
It resulted in increase of 20 % of hardness in aged HAMMCs when compared with as-cast HAMMCs. The highest hardness was noticed in composites for aged with 10%SiC+10%Al2O3
reinforcement. There is a gain in hardness of 20 % due to heat treatment in HAMMCs. In T6 heat treatment of HAMMCs, the thermal mismatching of matrix and reinforcement thermally promotes dislocation density improvement in dislocation densities outcome in advanced resistance to plastic deformation, led to better hardness. It is reported that the addition of SiC+alumina to Al7075 in metal-alloys lead to superior hardness number and strength.
After 10 % of reinforcement it is observed that for both the as-cast and age hardened conditions there is a decrement in hardness. This decrement is may be due to particle grouping in the surrounding matrix, which in turn it alter the hardness of material.
3.3 Analysis of variance (ANOVA)
In the present work, optimizing the parameters of the Al 7075/SiC/Al2O3 specimen is carried out
using the Taguchi method. Three parameters and three factors are considered to optimize the parameters. Factors considered are material composition, load and sliding distance. Loads considered are 2 kg, 4 kg, and 6 kg and material compositions considered are 5 %, 10 %, and 15 % of SiC/Al2O3 reinforcement in the Al7075
matrix. The experimental data i.e composition, load and sliding distance are input functions for the Taguchi design. For the given input functions, Taguchi design has been analyzed. The analysis outcomes are shown in Fig. 5a.
Fig. 5. Wear rate vs Composition, Load and Sliding Distance at the a) as-cast condition, and b) age hardened condition.
reduces up to 10 % of Sic/Al2O3 reinforcement in
the Al7075 matrix and increases for 15 % Sic/Al2O3.
From Fig. 5b it is seen that as sliding distance increases as wear rate decreases for the composite. It is obvious that as the increment in the applied load gives the increment in the wear. As composition increases wear rate decreases for 10 % of SiC/Al2O3 and increases by 15 % SiC/Al2O3.
The optimize composition is at 10% SiC/Al2O3
based on load, sliding distance, and composition of the Al7075- SiC/Al2O3 composites for both the
conditions age hardening and without age hardening treatment. From the Taguchi analysis, on the specimens, Al7075- 10%SiC/Al2O3 is the
optimized composition and wear rate reduces for the optimized composition.
ANOVA referred as analysis of variance utilizes the data from the Taguchi’s array. ANOVA techniques can be utilized to optimize the parameters and their performance behavior.
Analysis of variance in short called ANOVA is a statistical tool used to evaluate the level of the individual involvement of the process parameter on the responses such as sliding distance and load carrying capacity, and furthermore, give precisely the arrangement of the process parameters. Individual optimal values for the process parameters and their predefined performance attributes can be found. Table 2 shows the results of ANOVA for Load, composition and sliding distance.
From the ANOVA outcomes it is observed that, the factors affecting the wear rate are the composition (10.48 %), load (76.02 %) and sliding distance (13.05 %) at as cast condition and for age hardened condition the factors affecting the wear rate are the composition (0.29 %), load (52.52 %) and sliding distance (42.69 %).
Table 2a. ANOVA for Wear rate at as-cast condition.
Source DF Seq SS Adj MS Value F- Value P- %confi-dence level
Compo-sition 2 3.311 1.6558 23.19 0.041 10.48 Load 2 24.024 12.012 168.21 0.006 76.02 Sliding
Distance 2 4.123 2.0618 28.87 0.033 13.05
Error 2 0.142 0.0714 0.45
Total 8 31.602 100.00
Table 2b. ANOVA for Wear rate for aging condition.
Source DF Seq SS Adj MS Value F- Value P- %confi-dence level
Compo-sition 2 0.070 0.035 0.07 0.939 0.29 Load 2 12.545 6.272 11.67 0.079 52.52 Sliding
Distance 2 10.197 5.098 9.48 0.095 42.69
Error 2 1.075 0.537 4.50
Total 8 23.888 100.00
DF=Degrees of freedom, SS=sum of squares, MS=Mean Square, F=Variance & P= test statics.
The ANOVA analysis demonstrates that the wear rate of the material mainly influenced by load, sliding distance than the composition of the material. It is obvious that as load increases wear rate increases. Also, the factors affecting the wear rate are the sliding distance, and composition The ANOVA analysis demonstrates that wear rate of the material mainly influenced by the composition of the material and also by the load and sliding distance. It is obvious that as composition increases wear rate decreases, in turn, reduces the wear.
3.4 Microstructure of Worn Surface
The Figs. 6 and 7 shows that the surface morphology of as-cast and age hardened Al7075/SiC-Al2O3 HAMMCs respectively,
tested under ambient temperature with load and speed.
(a) As Cast-2kg-600rpm (b) As Cast-6kg-600rpm
(c) 5%-2kg-600rpm (d) 5%-6kg-600rpm
(e) 10%-2kg-600rpm (f) 10%-6kg-600rpm
(g) 15%-2kg-600rpm (h) 15%-6kg-600rpm Fig. 6. SEM Micrographs of worn surface of as-cast HAMMCs.
The micrographs show that a number of continuous grooves had appeared on the worn surface. These parallel grooves are the evidence of micro plugging and similar worn surfaces with increased severity were seen. Extensive plugging can be observed on the worn surfaces which indicate that prominent wear mechanism in the composites.
The reattachment of wear debris on the worn surfaces was also noticed. Composites exhibit the same worn surfaces after the 2 kg(19.62N), and 6 kg(58.86N). The wide and shallow grooves were noticed on the as-cast worn
surface of composites as shown in Fig. 6. Similar behavior was observed in age hardened composites shown in Fig.7. However in reinforced heat treated HAMMCs worn surfaces were relatively smooth fine grooves and at the edge of the grooves slight plastic deformation was observed in composite.
Micrographs reveal the smooth surface with fine ploughing grooves. Similar trend was obtained for other researchers who have studied on Al6061-Al2O3 and Al7075-SiC composites with
similar wear behavior [21,22]. The as-cast matrix alloy grooves on the worn surfaces were coarse and there is plastic deformation and the grooves edge is heavy when compared with the extruded matrix alloy .
Exhibits the grooves along the direction of the sliding and material delamination were observed on the worn surface of the hybrid composite. By increasing the reinforced material SiC and Al2O3 the grooves are reduced and some
smooth wear tracks could also be seen. Small size grooves are seen with oxide patches.
(a) Al7075-2kg-600rpm (b) Al7075-6kg-600rpm
(c) 5%-2kg-600rpm (d) 5%-6kg-600rpm
(g) 15%-2kg-600rpm (h) 15%-6kg-600rpm Fig. 7. SEM Micrographs of worn surface of age hardened HAMMCs.
3.5 Comparisons of wear behaviour: as-cast and age hardening conditions
For each condition of wear test, three specimens were tested and standard deviation is calculated. For the same error bars are added as shown in Figs. 8, 9 and 10.
Figure 8 shows the comparison of as-cast and age hardened HAMMCs for different load and at a sliding distance of 282.47 m. At lower loads, 2 kg (19.62 N), the contact resistance is high, due to which mild wear occurs. The rubbing surfaces form the fine wear debris which mainly consists of aluminum and FeO2. The rubbed face appears
to be polished.
Fig. 8. Influence of load on wear-rate at 252.47m.
The wear rate was uniform at medium loads, 4kg (39.24 N), the wear rate in as-cast, HAMMC and heat treated as cast, and heat treated HAMMC composite decreases. At higher loads, 6 kg (58.86 N), the contact resistance was low, leads to severe wear.
Figure 9 shows the comparison of as-cast and age hardened HAMMCs for different load and at a sliding distance of 565.48m. The wear rate of the heat treated composite decreases as
compared to as-cast condition. The oxide film formed on the wearing surface prevents the metal to metal contact. In as-cast and heat treated Al7075-10%Sic- 10%Al2O3 HAMMCs the
particulate acts to restrain the change to a severe wear rate. The wear rate of heat treated HAMMCs were lesser than that of HAMMCs.
Fig. 9. Influence of load on wear-rate at 565.48 m.
Figure 10 shows the comparison of as-cast and age hardened HAMMCs for different load and at a sliding distance of 848.23 m.
In the Metal Matrix Composites (MMCs) increase wt% of SiC+Al2O3 reinforcement improves the
hardness.. Addition of hard particulate reinforcement in the composites restricts the composites from getting soft. It results in reductions in the wear rate . It was observed that the volumetric wear rate decreased in heat treated HAMMCs with increased SiC+Al2O3 reinforcement and aging
When compared with the base alloy the weight loss was decreased in MMCs. In HAMMCs the weight loss was further reduced when compared with aged HAMMCs. Remarkably the lowest weight loss was observed in Al7075-10wt%SiC-10wt%Al2O3 with aged HAMMCs.
At 15 wt.% of reinforcement, it is observed that decrease of wear rate on increment of sliding distance. With increase of sliding distances tribo-oxidation intensify. More tribo-oxides results in the decrease of coefficient of friction and wear rate.
The incorporation of reinforcement materials in an aluminum alloy increases the load bearing capacity. The investigation of wear behaviour of Aluminum Matrix Composites (AMCs) against friction materials is receiving particular attention because of the possibility of using these materials for disc brakes in automotive application . The addition of reinforcement in an aluminium matrix increases the load bearing capacity and higher wear resistance. The role of SiC+Al2O3 reinforcement has proved to be
valuable in better wear resistance of the HAMMCS The improvement of resistance of wear of the hybrid composite is due to the adding up of SiC+Al2O3 reinforcement.
Higher wear rate and weight loss at 15 % reinforcement is due to agglomeration of reinforcement particles in the surrounding matrix.
From the investigation the following conclusions were drawn on the mechanical and wear performance of as-cast and age hardened HAMMCs.
1.Stir casting technique is an economically appropriate process for the production of HAMMC. The micro-structural study of SEM and XRD techniques shows the homogeneous distribution of the particulates in the hybrid composites.
2.From the Vickers’s hardness test, age hardened hybrid composite gain the hardness by 24 % for 10 wt.% reinforcement as compared with as- cast composites. 3.From the ANOVA, load is identified as the
main parameter, which influences the wear loss of composite by sliding distance and weight fraction of SiC and alumina.
4.The age hardened Al7075/ SiC+Al2O3 composite shows excellent resistance to wear as compared to as-cast hybrid composite.
5.As compared to base alloy, age hardened HAMMC has improved wear resistance properties.
I wish to thank University B.D.T. College of Engineering (Davangere), DST-PURSE Laboratory of Mangalore University, VGST-K FIST facility for melting and Material Testing (SJMIT, Chitradurga) for their support in providing facilities for various characterizations of materials and helped me to complete my research work.
 D.B. Miracle, S.L. Donaldson, ASM Handbook, Composites, vol. 21, ASM International, 2001.
 N. Stoloff, D. Alman, Innovative Processing Techniques for Intermetallic Matrix Composites. MRS Proceedings, vol. 194, pp. 31-43, 1990, doi: 10.1557/PROC-194-31
 J. Goni, I. Mitxelena, J. Coleto, Development of low cost Metal Matrix Composites for commercial Applications, Material Science and Technology, vol. 16, no. 7-8, pp. 743-746, 2000, doi: 10.1179/026708300101508739
 M. Singla, D.D. Dwivedi, L. Singh, V. Chawla,
Development of aluminium based silicon carbide particulate metal matrix composite, Journal of Minerals and Materials Characterization and
Engineering, vol. 8 no. 6, pp. 455–467, 2009, doi:
 K.R. Kumar, Aluminium/fly-ash composites Effect of particle size on mechanical properties and tribological behaviour of aluminium/fly-ash composites, Science and Engineering of Composite Materials, vol. 19, no. 3, pp. 247–253, 2013, doi: 10.1515/secm-2011-0139
 K. Komai, K. Minoshima, H. Ryoson, Tensile and
fatigue fracture behavior and water-environment effects in a SiC-whisker/7075-aluminum composite, Composites Science and Technology, vol. 46, no.
1, pp. 59–66, 1993, doi:
 R.L. Deuis, C. Subramanina, J.M. Yellup, Dry sliding wear of aluminium composites-a review, Composites Science and Technology, vol. 57, iss.
4, pp. 415-435, 1997, doi:
 V.C. Uvaraja, N. Natrajan, Comparison on Al6061
and Al7075 alloy with SiC and B4C reinforcement
hybrid metal matrix composites, Journal of
Minerals and Materials Characterization and Engineering, vol. 11, pp. 757-768, 2012.
 N. Radhika, R. Subramanian, V.S. Prasat,
Tribological Behaviour of Aluminium /Alumina/Graphite Hybrid Metal Matrix Composite using Taguchi’s Techniques, Journal of Minerals and Materials Characterization and Engineering, vol. 10, no. 5, pp. 427-443, 2011.  N. Radhika, R. Subramanian, V.S. Prasat, B.
Anandavel, Dry sliding wear behaviour of aluminium/alumina/graphite hybrid metal matrix composites, Journal of Industrial Lubrication and Tribology, vol. 64, iss. 6, pp. 359-366, 2012, doi:
 S. Doddamani, M. Kaleemulla, Y. Begum, K.J.
Anand, An Investigation on Wear Behavior of
Graphite Reinforced Aluminum Metal Matrix
Composites, Journal of Research in Science,
Technology, Engineering and Management,
Special issue, pp. 1-6, 2017.
 A.M. Rajesh, M. Kaleemulla, Experimental investigations on mechanical behavior of aluminium metal matrix composites, Materials Science and Engineering, vol. 149, 2016, doi: 10.1088/1757-99X/149/1/012121
 T. Bharath, A.M. Rajesh., M. Kaleemulla, K. Rangasravantha, Experimental investigations on mechanical and wear behavior of hybrid aluminium alloy, International Journal of Research in Engineering and Technology, vol. 5, iss. 13, pp. 128-131, 2016.
 A.M. Rajesh, M. Kaleemulla, Effect of heat treatment on hybrid aluminum metal matrix composites, International Journal of Emerging Research in Management & Technology, vol. 6, iss. 5, pp. 548-551, 2017.
 W.Q. Song, P. Kraulis, A.P. Mourrtz, S.
Bandyopadhyay, The effect of thermal ageing on the abrasive wear behaviour of age-hardening 2014 Al/SiC and 6061 Al/SiC composites, Wear,
vol. 185, iss. 1-2, pp. 125-130, 1995, doi:
 N. Radhika, Analysis of Three Body Abrasive Wear Behaviour of Centrifugally Cast Aluminium
Composite Reinforced with Ni Coated SiC using Taguchi Technique, Tribology in Industry, vol. 40, no. 1, pp. 81-91, 2018, doi: 10.24874/ti.2018.40.01.07
 M. Bai, Q. Xue, X. Wang, Y. Wan, Liu, Wear mechanism of SiCwhisker-reinforced 2024 al-alloy matrix composites in oscillating sliding wear tests, Wear, vol. 185, iss. 1-2, pp. 197-202, 1995, doi: 10.1016/0043-1648(95)06617-9
 M.K. Surappa, R.K. Uyyuru, S. Brusethaug, Effect of reinforcement volume fraction and size distribution on the tribological behaviour of Al-composite/brake pad tribocouple, Wear, vol. 260, iss. 11-12, pp. 1248–1255, 2006, doi: 10.1016/j.wear.2005.08.011
 ASTM G99-95, Standard Test Method for Wear Testing with a Pin-on-Disk Apparatus, Annual Book of ASTM Standard, 1995.
 T. Alpas, J. Zhang, Effect of SiC particulate reinforcement on the dry sliding wear of aluminum-silicon alloys (A356), Wear, vol. 155, iss. 1, pp. 83-104, 1992, doi: 10.1016/0043-1648(92)90111-K
 J.P. Tu, Y.Z. Yang, Tribological behavior of All8B4033-whisker reinforced hypoeutectic Al-Si-Mg-matrix composites under dry sliding conditions, Composite Science Technology, vol. 60, iss. 9, pp. 1801-1809, 2000, doi: 10.1016/S0266-3538(00)00067-1
 M.D. Kulkarni, P.S. Robi, R.C. Prasad, P.
Ramakrishna, Deformation and fracture behavior
of cast 7075Al-SiCp composites at room and elevated temperatures, Material Transactions, JIM,
vol. 37, no. 3, pp. 223-229, 1996, doi:
 A.A. Hamid, P.K. Ghosh, S.C. Jain, S. Ray, The influence of porosity and particles content on dry sliding wear of cast in situ Al(Ti)–Al2O3(TiO2)
composite, Wear, vol. 265, iss. 1-2, pp. 14-26, 2008, doi: 10.1016/j.wear.2007.08.018
 A.M. Rajesh, M. Kaleemulla, D. Saleemsab, Effect of addition of SiC and Al2O3 on wear behavior of hybrid aluminum metal matrix composites, Acta Technica Corviniensis – Bulletin of Engineering, vol. 12, iss. 1, pp. 43-52, 2019.
 M.J. Ghazali, W.M. Rainforth, M.Z. Omar, A comparative study of mechanically mixed layers (MMLs) characteristics of commercial aluminium alloys sliding against alumina and steel sliders,